Crystal structure of (C6H14N2)Sc4F2(PO4)4.4H2O
; Chemistry of Materials  (2004) –; doi:10.1021/cm048764r

data_4000493
_publ_section_title
;
Crystal structure of (C6H14N2)Sc4F2(PO4)4.4H2O
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/cm048764r
_journal_year                    2004
_chemical_formula_sum            'C6 H22 F2 N2 O20 P4 Sc4'
_chemical_formula_weight         783.98
_chemical_name_common            'scandium fluorophosphate'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 102.761(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.2826(16)
_cell_length_b                   12.6977(19)
_cell_length_c                   17.864(3)
_cell_measurement_reflns_used    2021
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      27.52
_cell_measurement_theta_min      1.98
_cell_volume                     2274.8(6)
_diffrn_ambient_temperature      173(2)
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_device_type  'Bruker SMART CCD'
_diffrn_measurement_method       ?
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0675
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            5236
_diffrn_reflns_theta_max         27.52
_diffrn_reflns_theta_min         1.98
_diffrn_standards_decay_%        ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_number         ?
_exptl_absorpt_coefficient_mu    1.539
_exptl_absorpt_correction_T_max  0.9410
_exptl_absorpt_correction_T_min  0.8019
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2000)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.289
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1576
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.04
_refine_ls_extinction_coef       ?
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     428
_refine_ls_number_reflns         5236
_refine_ls_number_restraints     289
_refine_ls_restrained_S_all      1.043
_refine_ls_R_factor_all          0.0605
_refine_ls_R_factor_gt           0.0418
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0390P)^2^+3.2242P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0981
_refine_ls_wR_factor_ref         0.1065
_reflns_number_gt                4072
_reflns_number_total             5236
_reflns_threshold_expression     >2sigma(I)
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      P21/n
_cod_database_code               4000493